Rev. February 5, 2007
MISSISSIPPI DEPARTMENT OF TRANSPORTATION
FIELD MANUAL For
HOT MIX ASPHALT (HMA)
MATERIALS DIVISION Rev. February 5, 2007
Rev. February 5, 2007 2
TABLE OF CONTENTS
Page CHAPTER 1: GENERAL 6 1.1 PURPOSE 6 1.2 TERMINOLOGY 6 1.3 DEFINITIONS 7 1.4 REFERENCED DOCUMENTS 8 CHAPTER 2: PERSONNEL REQUIREMENTS 11 2.1 GENERAL 11 2.2 CONTRACTOR QUALITY CONTROL PERSONNEL 11 2.3 MDOT QUALITY ASSURANCE PERSONNEL 11 CHAPTER 3: QC AND QA LABORATORIES 12 3.1 GENERAL 12 3.2 QC LABORATORY 12 3.3 QA LABORATORY 13 CHAPTER 4: JOB MIX FORMULA 14 4.1 GENERAL 14 4.2 CONTRACTOR RESPONSIBILITIES 14 4.2.1 Original Designs of Job Mix Formula 14 4.2.2 Job Mix Formula Transfers 14 4.2.3 Adjustments To Job Mix Formula 15 4.2.4 Redesign of Job Mix Formula 17 4.3 MDOT RESPONSIBILITIES 17 4.3.1 Original Designs 17 184.108.40.206 Project Engineer 17 220.127.116.11 District Materials Engineer 17 18.104.22.168 Central Laboratory 18 4.3.2 Job Mix Formula Transfers 18 22.214.171.124 Project Engineer 18 126.96.36.199 District Materials Laboratory 18 188.8.131.52 Central Laboratory 19 4.3.3 Adjustments To Job Mix Formula 19 184.108.40.206 Project Engineer and District Materials Laboratory 19 220.127.116.11 Central Laboratory 19
Rev. February 5, 2007 3
TABLE OF CONTENTS (Contd.)
Page CHAPTER 5: CONTRACTORS QUALITY MANAGEMENT PROGRAM 20 5.1 GENERAL 20 5.2 SAMPLING 20 5.2.1 Aggregate and RAP Stockpiles 20 18.104.22.168 Sampling Location 20 22.214.171.124 Sampling and Testing Frequency 20 126.96.36.199 Testing 20 5.2.2 Asphalt Binder Material 20 5.2.3 HMA Mixture 21 188.8.131.52 Testing Requirements 21 184.108.40.206.1 Mixture Gradation 21 220.127.116.11.2 Air voids and VMA 21 18.104.22.168.3 Asphalt Content 21 22.214.171.124.4 Fractured Face Count 22 126.96.36.199.5 Stripping Tests 22 188.8.131.52.6 Density Tests 22 184.108.40.206.7 Quality Control Charts 22 220.127.116.11 Determining Sampling Increment Size 22 18.104.22.168 Determining Sample Location 23 22.214.171.124 Mixture Sampling Point 24 126.96.36.199 Sample Identification 24 5.3 REDUCTION OF MIXTURE SAMPLES TO TESTING SIZE 24 5.3.1 General 24 5.3.2 Initial Sample 24 5.3.3 Nuclear AC / Moisture / Gyratory Reduction 25 5.3.4 MSG (Gmm) / Extraction Reduction 26 5.3.5 Modifications 26 5.4 COMPACTION OF SHRP GYRATORY SPECIMENS 27 5.5 COMPACTED SPECIMEN BULK SPECIFIC GRAVITY 28 5.6 MAXIMUM SPECIFIC GRAVITY, Gmm 29 5.7 MOISTURE DAMAGE TESTING 33 5.8 CALCULATING AIR VOIDS, Pa 34 5.9 CALCULATING VOIDS IN MINERAL AGGREGATE, VMA 35 5.10 GRADATION OF EXTRACTED AGGREGATE FROM MIXTURE 36 5.11 FIELD ADJUSTMENT OF JOB-MIX FORMULA, JMF 36 5.12 DOCUMENTATION 36 5.13 JMF LIMITS, WARNING LIMITS AND WARNING BANDS 36 5.14 CORRECTIVE ACTION 37 5.15 TROUBLE SHOOTING 39
Rev. February 5, 2007 4
TABLE OF CONTENTS (Contd.)
Page CHAPTER 6: MDOT QUALITY ASSURANCE PROGRAM 41 6.1 MATERIALS SAMPLES 41 6.1.1 Asphalt Binder Material 41 6.1.2 Hydrated Lime 41 6.2 HMA QUALITY ASSURANCE REQUIREMENTS 41 6.2.1 General 41 6.2.2 Samples 41 6.2.3 Testing Frequency 42 6.2.4 Quality Assurance Testing 42 6.2.5 Verification of Quality Control Test Results 42 6.3 HMA PLANT PRODUCTION REVIEW GUIDELINES 43 6.3.1 Prestart-up 43 6.3.2 Start-up Day 44 6.3.3 During Production 45 6.4 ROADWAY PRODUCTION REVIEW GUIDELINES 46 6.4.1 Placement Operations 47 6.4.2 Test Strip 48 6.4.3 Pavement Smoothness 48 6.5 REQUIRED PLANT SHUTDOWNS 48
6.6 GUIDELINES FOR RESOLUTION OF DIFFERENCES BETWEEN QC AND QA TEST RESULTS 49
Flow Chart 50 6.6.1 Examples of Resolution of Differences Between QC and QA Results 52 CHAPTER 7: ROADWAY DENSITY 58 7.1 PURPOSE 58 7.2 DEFINITIONS 58 7.3 ROADWAY DENSITY MEASUREMENTS 58 7.4 FIRST PRODUCTION DAY 58 7.5 COMPACTIVE EFFORT FOR LOT TO LOT OPERATIONS 61 7.6 NUCLEAR DENSITY PROCEDURE FOR DETERMINING
ACCEPTANCE OF LOTS 61 7.7 NUCLEAR GAUGE BIAS UPDATE 63 7.8 LIMITS ON DAILY COMPACTION 65 7.9 PROCEDURE FOR DETERMINING LIMITS FOR REMOVING LOT(S) OR PART(S) THEREOF NOT ALLOWED TO REMAIN IN
PLACE 66 7.10 PROCEDURE FOR RE-EVALUATING CORRECTED LOT 67
Rev. February 5, 2007 5
APPENDIX 1: MISSISSIPPI TEST METHODS and MDOT SOPs 69 APPENDIX 2: FORMS 116 APPENDIX 3: EXAMPLE PROBLEMS 128
Rev. February 5, 2007 6
CHAPTER 1 GENERAL
1.1 Purpose - The purpose of this manual is to establish uniform procedures and
practices for quality control and quality assurance sampling and testing of hot mix asphalt (HMA). This manual provides instructions and procedures for Contractor and MDOT personnel for the design, control and acceptance of asphalt mixtures under MDOTs Quality Management Program (QMP) as required by the specifications. Sampling procedures, sampling frequencies, and testing to be performed by the Contractor for the quality control of asphalt mixtures at the asphalt plant and by MDOT for the quality assurance and acceptability of these mixtures are detailed. When necessary for clarification, examples are provided. For ready reference, the specifications, standard operating procedures, and example forms for documentation of test results are provided in appendices to this manual.
AASHTO - American Association of State Highway and Transportation Officials. ASTM - American Society of Testing Materials. BRCF - Bulk Specific Gravity (Gmb) Reheat Calibration Factor CAT-I - Certified Asphalt Technician-Level I. Contractor or MDOT personnel who have successfully completed the MDOT HMA Technician Certification Program for Level I certification. This certification level is required for performance of sampling and testing of HMA mixtures and component materials. CAT-II - Certified Asphalt Technician-Level II. Contractor or MDOT personnel who have successfully completed the MDOT HMA Technician Certification Program for Level I and Level II. This certification level is required for Contractor personnel who interpret HMA test results and make necessary plant adjustments such that the HMA mixture produced conforms to the job mix formula. CMDT - Certified Mixture Design Technician. Contractor or MDOT personnel who have successfully completed the MDOT HMA Technician Certification Program for the design of HMA mixtures. This certification level is required for designing or approving the design of HMA mixtures. All personnel at this level must have first completed requirements and obtained CAT-I and CAT-II certification levels.
Rev. February 5, 2007 7
FHWA - Federal Highway Administration
HMA - Hot Mix Asphalt
HT - High Type Asphalt Mixtures
JMF - Job Mix Formula
MDOT - Mississippi Department of Transportation
MRCF - Maximum Specific Gravity (Gmm) Reheat Correction Factor
MT-## - Mississippi Test Methods (e.g., MT-78)
MT - Medium Type Asphalt Mixtures
NCAT - National Center of Asphalt Technology
QA - Quality Assurance
QC - Quality Control
QMP - Quality Management Program
RAP - Recycled Asphalt Pavement
ST - Standard Type Asphalt Mixtures
SUPERPAVE - Superior Performing Asphalt Pavement
TSR - Tensile Strength Ratio
VFA - Voids Filled With Asphalt
VMA - Voids In Mineral Aggregate 1.3 Definitions
Coarse Aggregate - Material retained on the No. 8 sieve. Check aggregate specific gravity test procedures for sample requirements.
Fine Aggregate - Material passing the No. 8 sieve. Check aggregate specific gravity test procedures for sample requirements.
JMF - The JMF of a mixture is defined as the combined gradation for the blended aggregate, the percentages of the various mixture components, the design asphalt binder content, and the mixture VMA.
Maximum Density Line - The maximum density line is a straight line plot on the FHWA 0.45 power chart which extends from the zero origin point of the chart through the plotted point of the combined aggregate gradation curve on the nominal maximum sieve size.
Nominal Maximum Sieve Size - The nominal maximum sieve size is one sieve size larger than the first sieve to retain more than 10 percent of the aggregate.
Maximum Sieve Size - Maximum sieve size is the smallest sieve at which 100 percent of the aggregate passes.
Rev. February 5, 2007 8
NInitial - The number of revolutions of the Gyratory Compactor representing the compactibility of the mixture received from the asphalt spreader. The required NInitial revolutions for a particular type mixture are specified in the contract specifications.
NDesign - The number of revolutions of the Gyratory Compactor required for design characteristics of the job mix formula. The required NDesign revolutions for a particular type mixture are specified in the contract specifications.
NMaximum - The number of required revolutions of the Gyratory Compactor representing the density of the pavement layer at the end of design life. The required NMaximum revolutions for a particular type mixture are specified in the contract specifications.
1.4 Referenced Documents
AASHTO Standards AASHTO M 92 Wire Cloth and Sieves for Testing Purposes AASHTO M 231 Weighing Devices Used in the Testing of Materials
AASHTO R 18 Establishing and Implementing a Quality System for Construction Materials Testing Laboratories
AASHTO T 2 Sampling of Aggregates AASHTO T 11 Materials Finer Than 75-m (No. 200) Sieve in Mineral
Aggregates by Washing AASHTO T 19 Unit Weight and Voids in Aggregate AASHTO T 27 Sieve Analysis of Fine and Coarse Aggregates AASHTO T 37 Sieve Analysis of Mineral Filler for Road and Paving Materials AASHTO T 40 Sampling Bituminous Materials AASHTO T 84 Specific Gravity and Absorption of Fine Aggregate
AASHTO T 85 Specific Gravity and Absorption of Coarse Aggregate AASHTO T 88 Particle Size Analysis of Soils AASHTO T 90 Determining the Plastic Limit and Plasticity Index of Soils AASHTO T 96 Resistance to Degradation of Small-Size Coarse Aggregate by
Abrasion and Impact in the Los Angeles Machine AASHTO T 104 Soundness of Aggregate by Use of Sodium Sulfate or
Magnesium Sulfate AASHTO T 166 Bulk Specific Gravity of Compacted Bituminous Mixtures
Using Saturated Surface-Dry Specimens AASHTO T 209 Theoretical Maximum Specific Gravity and Density of
Bituminous Paving Mixtures AASHTO T 218 Sampling Hydrated Lime
AASHTO T 269 Percent Air Voids in Compacted Dense and Open Bituminous Paving Mixtures
AASHTO T 275 Bulk Specific Gravity of Compacted Bituminous Mixtures Using Paraffin-Coated Specimens
AASHTO T 308 Determining the Asphalt Binder Content of Hot Mix Asphalt (HMA) by the Ignition Method
Rev. February 5, 2007 9
AASHTO Standards (Contd.)
AASHTO T 312 Preparing and Determining the Density of Hot Mix Asphalt (HMA) Specimens by Means of the Superpave Gyratory Compactor
AASHTO T 315 Determining the Rheological Properties of Asphalt Binder Using a Dynamic Shear Rheometer (DSR)
AASHTO T 316 Viscosity Determination of Asphalt Binder Using Rotational Viscometer
ASTM C 604 Test Method for True Specific Gravity of Refractory Materials by Gas-Comparison Pycnometer
ASTM C 1252 Test Method for Uncompacted Void Content of Fine Aggregate (as Influenced by Particle Shape, Surface Texture, and Grading)
ASTM D 3289 Standard Test Method for Density of Semi-Solid and Solid Bituminous Materials (Nickel Crucible Method)
ASTM D 3665 Standard Practice for Random Sampling of Construction Materials
ASTM D 4791 Standard Test Method for Flat Particles, Elongated Particles, or Flat and Elongated Particles in Coarse Aggregate
ASTM D 5821 Standard Test Method for Determining the Percentage of Fractured Particles in Coarse Aggregate
Mississippi Test Methods
MT-6 Nuclear Determination of Bitumen Content of Bituminous
Paving Mixtures MT-16 Nuclear Method for Field In-Place Density Determination MT-24 Determination of the Specific Gravity of Fine Aggregate Using
the Le Chatelier Flask MT-31 Quantitative Analysis of Hot Bituminous Mixtures MT-59 Determination of Loss of Coating of HMA (Boiling Water
Test) MT-63 Resistance of Bituminous Paving Mixtures To Stripping
(Vacuum Saturation Method) MT-76 Microwave Method for Determining the Moisture Content of
Hot Bituminous Mixtures MT-78 Volumetric Design of Hot Bituminous Paving Mixtures Using
The Superpave Gyratory Compactor
Rev. February 5, 2007 10
Standard Operating Procedures CSD-50-70-54-000 Random Sampling Forms TMD-004 Asphalt Paving Inspectors Daily Report TMD-005 QA Mixture Report TMD-006 Summary Report of QC Mixture Properties TMD-008 Summary Report of QC Gradation Properties TMD-020 HMA Daily Plant Samples Random Numbers TMD-042 Bituminous Mix Design QMP Inspectors Checklist Asphalt Roadway Inspection Checklist Asphalt Plant Inspection Checklist
Rev. February 5, 2007 11
CHAPTER 2 PERSONNEL REQUIREMENTS
2.1 General. MDOTs QMP program for HMA requires the performance of quality
control and quality assurance sampling, testing, and design by trained and knowledgeable personnel. Contractor personnel and MDOT personnel directly involved in QC and QA sampling and testing of HMA mixtures must have successfully completed the MDOT HMA Technician Certification Program (Materials Division Inspection, Testing, and Certification Manual Section 1.3.3) to obtain certification at the level commensurate with their duties.
2.2 Contractor Quality Control Personnel Requirements.
2.2.1 CAT-I Technician. The Contractor must provide at least one CAT-I Technician full time at each plant site during production and testing of HMA. Sampling of HMA and component materials must be conducted by the CAT-I Technician or by plant personnel under the direct observation of the CAT-I Technician. All testing, data analysis and data posting must be performed by the CAT-I Technician or by an assistant under the full time direct supervision of the CAT-I Technician. 2.2.2 CAT-II Technician. The Contractor must have a CAT-II Technician available to make necessary process adjustments. 2.2.3 CMDT Technician. All job mix formulas submitted by the Contractor for approval must be developed by and signed by a CMDT Technician.
2.3 MDOT Quality Assurance Personnel Requirements.
2.3.1 CAT-I Technician. All sampling, testing and data analysis for quality assurance must be performed by a MDOT CAT-I Technician or by an assistant under the direct full time supervision of the MDOT CAT-I Technician. 2.3.2 CMDT Technician. A MDOT CMDT Technician must approve all proposed changes to the Contractors job mix formula.
Rev. February 5, 2007 12
CHAPTER 3 QC AND QA LABORATORIES
3.1 General. All laboratories involved in the design, design verification, quality control,
and quality assurance testing of asphalt mixtures and component materials must be fully equipped to perform the required tests. All such equipment must meet the requirements of MDOTs specified test methods.
3.2 QC Laboratory. Post an organization chart, including names, telephone numbers
and current certification (CAT-I, CAT-II and CMDT), of all personnel responsible for the quality control program on the project. Post the chart in a readily visible location.
Post all required quality control charts in a readily visible location, and maintain in an up-to-date status. Charts may be maintained on a computer. However, updated computer charts shall be printed and displayed at a minimum of once each production day.
The laboratory shall be setup and calibrated prior to production. Calibration shall be according to the procedures and frequencies given in AASHTO R 18. Inspect and calibrate the laboratory equipment as follows:
Check calibration of Gyratory compactor according to the requirements in the manufacturers manual (at a minimum, verify the angle of gyration and the load on the specimen during compaction). Check balances for accuracy, precision and readability in accordance with AASHTO M 231. Check the water baths used for specific gravity testing for constant water level, temperature, and make sure the specimen basket does not touch the walls of the tank each time testing is performed. Make sure a non-corrosive metal wire or a non-absorptive cord is used to hang the basket from the bottom of the balance. Check calibration of maximum specific gravity flask and fine aggregate angularity cylinder. Check vacuum pumps to confirm that the required pressure is being applied to the flask or pycnometer. Check accuracy of all thermometers. Check temperature of ovens and water baths.
Rev. February 5, 2007 13
Check sieves for conformance to AASHTO M 92. As a daily routine during use, visually check sieves for holes, wear and separated or broken mesh. Ensure inside diameter of gyratory molds meets tolerances specified in Section 4.2 of AASHTO T 312. Molds found to be outside the tolerance should be discarded.
Maintain a written record of all calibration data in the laboratory files. 3.3 QA Laboratory. Post a chart in the QC Laboratory and in the QA Laboratory
giving the names, telephone numbers and current certification (CAT-I, CAT-II and CMDT) for all personnel responsible for the quality assurance program on the project(s). Calibrate all laboratory equipment according to the requirements for the QC laboratory in Section 3.2 of this manual. At the beginning of production, and randomly thereafter, inspect measuring and testing devices in the QC Laboratory to confirm both calibration and condition. Document all inspections made. Promptly notify the Contractor, both verbally and in writing, of any deficiencies found. Refer any questions on proper equipment or calibration to the Materials Division for resolution.
Rev. February 5, 2007 14
CHAPTER 4 JOB-MIX FORMULA
4.1 General. The Contractor is responsible for the design of each job mix formula used
on the project and for any necessary adjustments during production. A job mix formula may be a new design, or one being transferred from a previous project for which it was developed and under the conditions set out in the specifications. The Contractor shall not place any mixture prior to receiving a tentative approval for the job mix formula and a MDOT design number from the Central Laboratory. MDOT is responsible for the verification of each job mix formula submitted by the Contractor for use on the project.
4.2 Contractor Responsibilities. 4.2.1 Original Design of Job Mix Formula. Design the job mix formula in accordance with MT-78. At least 10 working days prior to the proposed use of each mixture, submit in writing to the Engineer (with a copy to the District Materials Laboratory) the proposed job mix formula signed by a CMDT Technician. Prepare samples of the materials representative of the job mix formula for submission to MDOTs Central Laboratory in accordance with MT-78.
4.2.2 Job Mix Formula Transfers. A verified job mix formula may be transferred from one project to another under the following conditions:
If the mixture is currently being produced on the project from which it is being transferred, check the quality control test results and the quality assurance test results to verify consistent performance to the job mix tolerances. If the test results show satisfactory performance, the job mix formula may be transferred. A summary of the results on MDOT Forms TMD-006 and TMD-008 shall be provided along with information on which projects the job mix formula had previously been used. If the mixture is not currently being produced on an active project or has not been produced within the past six months, run the bulk specific gravity test on each aggregate component. If the specific gravity of each individual aggregate component is within a tolerance of 0.025 from the original job mix formula, the combined bulk specific gravity of the aggregate blend is within a tolerance of 0.015 from the original job mix formula, and the mixture properties meet the design requirements when calculated with the new aggregate specific gravity results, the job mix formula may be transferred. At least 10 working days prior to the proposed use of each mixture, submit in writing to the Engineer (with a copy to the District Materials Laboratory) a
Rev. February 5, 2007 15
request for transfer of the verified job mix formula signed by the Contractors CMDT Technician. The written request must certify that the source and characteristics of the materials have not changed since the original job mix formula was issued. Include all required supporting documentation with the request. Original Job Mix Formulas that have been revised in the field during production as set out below in Subsection 4.2.3 of this manual shall not be transferred to another project. Only the revised JMF will be considered for transfer.
4.2.3 Adjustments To Job Mix Formula. When necessary, minor adjustments may be made to a job mix formula under the conditions set out in Subsection 401.02.5.7 of the contract specifications and as follows: Each job mix formula proposed and verified from laboratory tests is considered tentative until a sufficient quantity of mixture has been processed through the plant, placed on the roadway, compacted to required density, and tested to determine if any corrections or adjustments are needed. Determine what adjustments, if any, are necessary from the quality control test results and the quality assurance test results for density, VMA, air voids, asphalt content, aggregate gradation, and other required design characteristics. Check the specifications to determine the amount of RAP allowed in the mixture is not exceeded. This amount may be a function of mixture type and location in the structure (i.e.,. top lift). Check the aggregate blend for the proposed JMF to make sure that the Sand Ratio is less than or equal to 60 percent. Calculate the Sand Ratio by using the following formula:
Where: B = % of JMF passing the No. 30 sieve. C = % of JMF passing the No. 8 sieve. D = % of JMF passing the No. 200 sieve.
Rev. February 5, 2007 16
Example: JMF Gradation Sieve Size Percent Passing 1/2 100.0 3/8 96.5 No. 4 70.1 No. 8 42.4 No. 16 27.2 No. 30 19.8 No. 50 12.4 No. 100 8.3 No. 200 6.3
ts)Requiremen (Meets . - .. - . Ratio Sand 4.371003644236819
For surface course mixtures, check that the combined aggregate blend meets the specification limits for the amount of limestone used in the mixture (maximum of 30 percent of the total aggregate blend). For 9.5 mm mixtures, and all MT and HT mixtures designed above the maximum density line, check the fine aggregate angularity in accordance with ASTM C 1252, Method A. Check that the limits on the amount of natural sand in the mixture are not exceeded.
In the event adjustments are necessary, the change in aggregate gradation and asphalt content must be within the tolerances specified for the job mix formula (JMF limits) in Subsection 401.02.5.5 of the specifications when compared to the original JMF for the project. Regardless of such tolerances, any adjusted job mix formula gradation must be within the design master range in Subsection 401.02.1.2.3 of the specifications for the mixture specified. The job mix formula asphalt content may only be reduced if the production VMA meets or exceeds the minimum design VMA in Subsection 401.02.3.1.1 of the specifications for the mixture being produced.
When a job mix formula adjustment is necessary, submit a written request to the Engineer (with a copy to the District Materials Laboratory) signed by a CAT-II Technician, setting out what adjustments are needed. Attach sufficient test data to justify the change (current stockpile gradations, production results, aggregate specific gravities, and TSR data if necessary). The request must include the sample test number that indicates when the change is to become effective. The requested change, if approved, may become effective at a test point up to four individual tests prior to the test when the request was formally made. Written documentation in the form of a letter, FAX, or e-mail must exist indicating that the QC/QA team had
Rev. February 5, 2007 17
discussed a possible change for the adjustment to be allowed at a point prior to the test number at the time of the formal request. Further adjustments after the approval of a JMF change will not be allowed until at least six additional tests (at normal sampling frequency) have been conducted. 4.2.4 Redesign of Job Mix Formula. A job mix formula must be redesigned when any of the following events occur: (1) a change in sources of material(s) is made, (2) when unsatisfactory results or changed conditions make it necessary (such as segregation, bleeding, shoving, rutting, raveling, cracking, or other pavement distress), or (3) if the viscosity at 275F of the asphalt binder shipped changes by 50 percent or more in either direction from that used in the mix design, as evidenced by a comparison of the temperature-viscosity curves.
4.3 MDOT Responsibilities. MDOT is responsible for verification of Contractors job mix formulas in accordance with the following requirements: 4.3.1 Original Designs. 188.8.131.52 Project Engineer. Check the Contractors request to insure conformance to the bid items in the contract. If the request does not conform to the mixture type set out in the bid items, reject the request and return to the Contractor by cover letter explaining the reason for rejection. If the Contractors request is in conformance with the bid items, forward the request to the District Materials Engineer. 184.108.40.206 District Materials Engineer. Check the source for each coarse aggregate component and determine if it is from a MDOT approved source. If not, for each unapproved aggregate component obtain a 45 kg sample from the Contractors stockpile or cold feed bin in accordance with AASHTO T 2 and submit to the Central Laboratory for soundness and abrasion tests. Verification of the contractors job mix formula cannot be made until the aggregate sources are approved. Check the source of asphalt binder for listing on MDOTs Approved List of Suppliers. Asphalt binder from unapproved suppliers cannot be used. Check the Contractors proposed job mix formula for accuracy, completeness and conformance to the required design characteristics of the specifications. If in agreement, submit a written request to the State Materials Engineer for verification of the Contractors job mix formula. Attach a copy of the Contractors request, proposed job mix formula, and supporting data. Send a copy of your request with attachments to the Construction Division.
Rev. February 5, 2007 18
Deliver or have the Contractor deliver the samples required in MT-78 to the Central Laboratory. 220.127.116.11 Central Laboratory. Check the Contractors job mix formula for accuracy and conformance to design characteristics required in the specifications for the required HMA mixture. Check to see if each coarse aggregate component is from an approved source. If not, check for sample(s) from the District Materials Laboratory for source approval. Test the sample(s) in accordance with AASHTO T 19, T 96 and T 104, and determine conformance to Section 703 of the Standard Specifications. Test Contractor samples submitted with the job mix formula, in accordance with current MDOT policy. If all test results are found to be in conformance with the specification requirements, issue the verified job-mix formula on Form TMD-042 by cover letter. If the mixture is found not to be in conformance with the specification requirements, reject the job mix formula with an explanation of the reasons for the rejection in writing. 4.3.2 Job Mix Formula Transfers. 18.104.22.168 Project Engineer. Determine if the original job mix formula complies with the bid items in the contract for which the transfer is to be made. If the request does not conform to the mixture type set out in the bid items, reject the request and return to the Contractor by cover letter explaining the reason for rejection. If the Contractors request is in conformance with the bid items, forward the request to the District Materials Engineer.. 22.214.171.124 District Materials Laboratory. Verification of the Contractors request for transfer of a job mix formula from one project to another will be based on the Contractors documentation, and such additional testing and investigation that may be necessary. Verify that the source and characteristics of the materials have not changed since the original job mix formula was issued. Perform any additional testing and investigation that may be necessary for verification. If it is determined that there has been a change in the source of any component material(s) or there has been a change in any characteristics of the material(s) or mixture, reject the Contractors request in writing giving the reasons for rejection. When the investigation confirms that the source and characteristics of materials has not changed, the requested transfer may be made. The District Materials Engineer must submit a written request for the transfer to the State Materials Engineer. This
Rev. February 5, 2007 19
request must certify to the conditions set out in Subsection 4.2.2 of this manual for verification of job mix formula transfers. 126.96.36.199 Central Laboratory. Upon receipt of the District Materials Engineers request, check all documentation for conformance to specified requirements for verification of job mix formulas as set out in Subsection 4.2.2 of this manual. If the request meets the specified criteria, issue the verified job mix formula on Form TMD-042 and make distribution by cover letter. NOTE: All JMF transfers are once again tentative until production and compaction requirements for the new project are met. 4.3.3 Adjustments To Job mix Formula. 188.8.131.52 Project Office and District Materials Laboratory. Upon receipt of the Contractors request and documentation for adjusting the job mix formula, check to see if sufficient quantity of material has been processed through the plant, placed on the roadway, compacted, and tested in order to determine if adjustments are necessary (minimum of four QC production tests). From the Contractors documentation, determine if density, VMA, air voids, asphalt content, and other required design characteristics have been established by quality control test results and quality assurance test results. Determine if current production values meet the mixture design requirements. Determine if the requested adjustments to aggregate gradation and/or asphalt binder content are within the specified tolerances. (Note- The asphalt binder content can only be reduced if the production VMA meets or exceeds the minimum design VMA requirements for the mixture being produced.) If in agreement with the Contractors request, the District Materials Engineer shall submit a written request to the State Materials Engineer for a revised job mix formula with the Contractors request and all documentation attached. If not in agreement, reject the request and provide reasons for rejection in writing. 184.108.40.206 Central Laboratory. Review the request, and if warranted by the documentation, issue a revised job mix formula on Form TMD-042. Make distribution of the revised job mix formula by cover letter.
Rev. February 5, 2007 20
CHAPTER 5 CONTRACTORS QUALITY MANAGEMENT
PROGRAM 5.1 General. The Contractor is responsible for quality management and maintenance of
a quality control system that furnishes reasonable assurance that the mixtures and all component materials incorporated in the work conform to contract requirements. The Contractor is responsible for the initial determination and all subsequent adjustments in proportioning materials used to produce the specified mixture. Adjustments to plant operation, spreading, and compaction procedures must be made immediately by the Contractor when results indicate that they are necessary.
5.2.1 Aggregate and RAP Stockpiles. 220.127.116.11 Sampling Location. Obtain samples from the stockpiles or cold feed bins in accordance with AASHTO T 2. 18.104.22.168 Sampling and Testing Frequency. Take the first sample of each stockpile after the stockpiles have been established at the hot-mix plant and prior to the first day of mixture production. Thereafter, sample once every eight production samples with a minimum of one from each stockpile per production week. Stockpile testing of the aggregate and RAP piles during production will be waived provided that gradation tests were conducted during the building of the stockpiles (see Subsection 401.02.5.3 of the contract specifications). 22.214.171.124 Testing. Determine the washed gradation of each aggregate stockpile sample in accordance with AASHTO T 11 and T 27. Determine the gradation of RAP stockpile samples in accordance with MT-31. Determine the asphalt content of the RAP stockpile when necessary using the same procedures used for the design of the mixture (MT-78). For all 9.5 mm mixtures, and all MT and HT mixtures designed above the maximum density line, determine the fine aggregate angularity of the aggregate blend in accordance with ASTM C 1252, Method A. Conduct the tests in an area of the laboratory not subjected to vibration. This test may be conducted off site. 5.2.2 Asphalt Binder Material. Asphalt binder is accepted in accordance with the procedures set out in the Materials Division Inspection, Testing, and Certification Manual Section 2.1.2..
Rev. February 5, 2007 21
Asphalt binder from the asphalt working tank shall be sampled by the Engineer in accordance with AASHTO T 40 and ASTM D 3665. Samples will be obtained on a random basis at the minimum frequency of one sample per 200,000 gallons. The Contractor shall make available to the Engineer the samples, which shall be placed in a sealed one-quart metal container, for submission to the Central Laboratory for AASHTO T 315 testing. Immediately upon notification by MDOT that a sample of asphalt binder failed to conform to specification requirements, suspend operations. Notify the supplier and jointly determine the cause of the failure and take appropriate action to correct the problem. When it is determined that the asphalt binder is back in compliance, operations may resume. Any mixture placed containing non-complying asphalt binder will be accepted, removed, or replaced as appropriate in accordance with Subsection 105.03 of the Mississippi Standard Specifications for Road and Bridge Construction. 5.2.3 HMA Mixture. 126.96.36.199 Testing Requirements. As a minimum, the Contractors Quality Management Program (QMP) must include the following: 188.8.131.52.1 Mixture Gradation. Conduct extraction tests for gradation determination on the mixture. Sample according to the frequency set out in Subsection 401.02.5.3(i) of the contract specifications and test in accordance with MT-31. The minimum sample sizes for the mixtures are as follows:
Mixture Type Minimum Sample Size - gm 25 mm 3,000 19 mm 2,000
12.5 mm 1,500 9.5 mm 1,000
184.108.40.206.2 Air Voids and VMA. Determine air voids and VMA, at NDesign, from the average results of two bulk specific gravity tests on laboratory compacted specimens and two maximum specific gravity tests on the mixture. Sample according to the sample frequency set out in Subsection 401.02.5.3(i) of the contract specifications and test according to Sections 5.4 through 5.10 of this manual. 220.127.116.11.3 Asphalt Content. Determine the asphalt content in accordance with MT-6 (nuclear gauge) or by using the incinerator oven in accordance with AASHTO T 308. Sample according to the sampling frequency set out in Subsection 401.02.5.3(i) of the contract specifications.
Rev. February 5, 2007 22
18.104.22.168.4 Fractured Face Count. Determine fractured face count of aggregates retained on the No. 4 sieve in accordance with ASTM D 5821, at a minimum of one test per day of production. A face will be considered a fractured face only if it has a projected area of at least as large as one quarter of the maximum cross-sectional area of the aggregate particle, and the face has sharp and well-defined edges. This area will be visually determined. A piece of aggregate with a small chipped area will not be considered as having a fractured face. 22.214.171.124.5 Stripping Tests. At least one stripping test (TSR) must be performed according to MT-63 at the beginning of each job mix production and thereafter, one test per each two weeks of production. One stripping test (boiling water test) per day of production must be performed in accordance with MT-59. 126.96.36.199.6 Density Tests. Conduct density tests as necessary to control and maintain required compaction according to MT-16, Method C (nuclear gauge), or AASHTO T 166. (NOTE: The nuclear gauge may be correlated, at the Contractors option, with the average of a minimum of four pavement sample densities.) 188.8.131.52.7 Quality Control Charts. Plot the individual test data, the average of the last four tests, the warning limits and the JMF limits for the following characteristics as a minimum. Mixture Gradation (Percent Passing) Sieves:
1/2-in, 3/8-in, No. 8, No. 30, No. 16 (for 4.75 mm mixtures), and No. 200.
Asphalt Content, Percent - Pb Maximum Specific Gravity - Gmm Air voids @ NDesign, Percent - Pa VMA @ NDesign, Percent Keep charts up-to-date and posted in a readily observable location. Note any process changes or adjustments on the Air Voids chart. Charts may be maintained on a computer. However, updated computer charts shall be printed and displayed at a minimum of once each production day. 184.108.40.206 Determining Sampling Increment Size. At the beginning of each day, the Contractor shall specify the anticipated tonnage to be produced. The frequency of sampling is then determined from Section 401.02.5.3(i) of the contract specifications. The anticipated tonnage shall be split into appropriate testing increments and a sample obtained randomly from each increment. Complete MDOT Form TMD-020 for each production day.
Rev. February 5, 2007 23
EXAMPLE Anticipated Tonnage For The Day (Estimate)-------------------------------1800 Tons Number of Samples Required ------------------------------------------------ 3 Testing Increment Size (1800 3)--------------------------------------------- 600 Increment for Sample 1----------------------------------------------From 1 to 600 Tons Increment for Sample 2------------------------------------------From 601 to 1200 Tons Increment for Sample 3----------------------------------------From 1201 to 1800 Tons Increment for Sample 4----------------------------------------From 1801 to 2400 Tons 220.127.116.11 Determining Sample Location. The approximate location of each sample within the increments shall be determined by selecting random numbers according to S.O.P. CSD-50-70-54-000, or from Table 1 of ASTM D 3665 according to the procedures in Sections 5.2 through 5.6. At the start of the first day, select four (4) random numbers from a randomly selected starting point on one of the charts. For subsequent days, select four new random numbers by continuing from the ending number of the previous day in the same direction established when the initial numbers were chosen. Keep a copy of the chart in the project files. The calculations of sampling tonnage are completed for all four random numbers even though the Contractor predicted that only three tests would be required. This is done just in case the Contractors production exceeds the original prediction. The random numbers selected shall be multiplied by the tonnage increments selected for the day. This number shall then be added to the total tonnage of all previous increments to yield the approximate tonnage when the sample is to be taken. If this procedure calls for the first sample to be taken at less than 50 tons production, take the first sample at 50 tons production.
EXAMPLE (Increment Size From Example In Subsection 18.104.22.168)
Tonnage Random Increments + Total Tons Sample Sample Range Number x Random No. Prev. Increm. Tonnage 1 1 - 600 0.570 342 + 0 342 2 601 - 1200 0.351 211 + 600 811 3 1201 - 1800 0.656 394 + 1200 1594 4 1801 - 0.200 120 + 1800 1920 This procedure is to be used for any number of samples per day. The plant operator shall not be advised ahead of time when any of the samples are to be taken.
Rev. February 5, 2007 24
22.214.171.124 Mixture Sampling Point. Sample all mixture samples from the truck box. Truck box sampling presents some safety hazards because it may be necessary to climb on top of the truck box and stand on the hot mixture while sampling in order to obtain a representative sample. After the last batch has been dumped into the truck box, establish a reference point on the surface of the load, either at the high point, if some semblance of a conical shape exists, or near the middle of the truck box if the surface shows no such conical shape. Then establish at least three incremental sample points about midway between the previously established point and the sides to the truck and equally spaced around the load (see sketch). At these sampling points, remove the upper 2 to 3 inches of mixture, insert the sampling shovel or other device into the mixture to extract the sample increments and place increments in a sample container. The total sample shall have a mass of at least 40 kg. X - Reference Point A A - Sample Point B X B - Sample Point C C - Sample Point 126.96.36.199 Sample Identification. Bag/Box and label the retained portion of all samples. The label shall include: State or Contractors sample. Project ID. Date sample was taken. Sample No. Sample tonnage point. Percent AC being metered into the mixture at time the sample was taken. Mixture Type Designation being produced. Pavement layer being placed. Percent RAP setting at the time sample was taken, when applicable.
5.3 Reduction of Mixture Samples to Testing Size 5.3.1 General. The entire sample shall be mixed and quartered on a clean, smooth, metal surfaced table, with a minimum surface of 48 inches x 48 inches (it is recommended that this table be heated). 5.3.2 Initial Sample. Quarter the sample into State and Contractor samples. Start with the total minimum 40 kg of mix. Place entire sample on table, quickly mix and quarter to minimize temperature loss. Quarter sample as shown in the following sketch:
Rev. February 5, 2007 25
A B State Contractor 40+ kg
Contractor State Combine diagonal quarters as indicated on the sketch to form the State sample (A & D) and the Contractor sample (B & C) for further quartering. Continue quartering process until test samples are in the oven. Place in a closed container and label the retained sample with the required information in Subsection 188.8.131.52 of this manual. Store samples in a safe place until no longer needed for sample verification. Retain the State sample (A&D) (minimum of 20+ kg) in a dry and protected location at the laboratory site. Retain these samples until picked up by MDOT for the dispute resolution process (if needed) or 14 calendar days, whichever occurs first. At the completion of the project, the remaining samples may be discarded with the approval of the Engineer. 5.3.3 Nuclear AC / Moisture / Gyratory Reduction. Reduce the 20+ kg of mix from Subsection 5.3.2 of this manual into a Gyratory sample and a Nuclear AC / Moisture sample or retained sample according to the following sketch:
A B Gyratory (Gmb)Tests Nuclear AC/Moisture & Mix Tests 20+ kg C D Nuclear AC/Moisture Gyratory (Gmb)Tests & Mix Tests
Rev. February 5, 2007 26
Combine quarters B & C and place the unconsolidated material in the oven in a metal container at 10 to 20F above AC content gauge calibration temperature. If this sample is going to also be used for the maximum specific gravity test (Gmm), age for a period of time as required in Subsection 5.4.2. After oven aging, remove a portion of the combined quarters B&C for moisture test. Prepare a Nuclear AC test pan from remainder. After completion of AC content testing, quarter the sample as recommended in Subsection 5.3.4. For 19 mm and 25 mm mixtures, it will be necessary to save that part of segments B & C not used for the AC content gauge sample for recombining with the AC content gauge sample after the test to provide sufficient sample size for the Maximum Specific Gravity tests. Carefully reduce quartered A & D independently to the required specimen weight to produce 115 mm high gyratory specimens. Place in separate containers and age in the oven as required in Subsection 5.4.2. 5.3.4 MSG (Gmm) / Extraction Reduction. After completion of the Nuclear AC test, remove the mixture from the pan and quarter for further testing according to the following sketch:
A B MSG (Gmm) Specimens Extraction Testing 7 kg C D Extraction Testing MSG (Gmm) Specimens
For 19 mm and 25 mm mixtures, it will be necessary to save that part of the split in Subsection 5.3.3 not used for the AC content gauge sample for recombining with the AC content gauge sample after the test to provide sufficient sample size for the Maximum Specific Gravity tests. Combine quarters B&C for the extraction test. Careful handling of the materials is required to prevent possible segregation which may have a significant effect on the gradation results. Use quarters A & D independently for the Maximum Specific Gravity samples. Use the appropriate sample size as required in Subsections 184.108.40.206.1 and 220.127.116.11.
5.3.5 Modifications. Modifications to the above quartering process may be made depending on the testing options selected. Make the proposed changes to the process prior to the start of the project and with the approval of the Engineer. In no case will scooping from the bucket or a pile on the table be acceptable.
Rev. February 5, 2007 27
5.4 Compaction of SHRP Gyratory Specimens
5.4.1 Equipment 18.104.22.168 Compactor. The compactor shall conform to the SHRP Superpave Gyratory Compactor requirements in AASHTO TP 4. The compactor shall be located in an indoor controlled temperature environment. The angle of gyration shall be set at 1.25 0.02 using the manufacturers calibration kit furnished with the compactor. The compactor shall be set to apply a constant vertical load of 600 18 kPa. Set dwell at the appropriate number of gyrations or dwell time (this is typically 5 gyrations for most Troxler compactors, or 5 seconds for most Pine compactors). Other manufacturers are similar, but check with the MDOT Central Laboratory if uncertain. 5.4.2 Procedures. At least 30 minutes to one hour before compacting Gyratory specimens, place two specimen mold assemblies in the aging oven to heat up. The mold assembly consists of the specimen mold and puck. From the two samples of material obtained as described in Subsection 5.3.3 weigh approximately 4500 g (adjust weight to provide a compacted specimen approximately 115 mm (5 mm) in height) into a metal container, cover and place in a convection aging oven set at 10 to 20F above the compaction temperature. The compaction temperature shall be the temperature to which the asphalt binder must be heated to produce a kinematic viscosity of 280 30 mm2/s. The temperature will be determined from a current temperature-viscosity curve for the particular asphalt binder being used. (NOTE: For polymer modified asphalt binder, use the manufacturers recommended compaction temperature.) Mixture Aging (to allow for asphalt absorption and control compaction temperature): Heat the two covered containers of mixture for a minimum of 30 minutes not to exceed two (2) hours. These times may be increased for projects with extended storage or haul times. Place a paper disc in the bottom of the heated specimen mold assembly. Remove one container of mixture from the oven, pour the mixture into the mold using a funnel with one continuous operation, scrape the container and level the mixture in the mold. Measure temperature of the mixture in the mold. If within the compaction temperature range, place a paper disc on top of the mixture and compact immediately. If too hot, allow sufficient time to cool to the required temperature range. Do not allow the thermometer to touch the mold. Seat the mold assembly in the compactor and apply the number of gyrations required for NDesign according to mixture design requirements in Subsection 401.02.3.2 of the specifications for the mixture being produced.
Rev. February 5, 2007 28
After compaction is complete, remove the mold assembly from the compactor, remove the paper disc from the top of specimen, cool for 5 to 10 minutes in front of a fan before extruding the specimen. After cooling, extrude the specimen by using the hydraulic jack and holder furnished with the compactor. Smooth rough edges with spatula, place flat side down on a smooth and level surface, properly identify, and cool with a fan to room temperature. Repeat the above procedure for compaction of one additional specimen.
5.5 Compacted Specimen Bulk Specific Gravity, Gmb
5.5.1 Determine bulk specific gravity (GmbMeasured) at NDesign in accordance with AASHTO T 166, Method A. Weigh the specimens in air, designate this mass as A. Immerse the specimens in 77 2F water bath for 3 to 5 minutes and then weigh in water, designating this mass as C. Surface dry the specimens by blotting quickly with a damp towel and then weigh in air (include any water that may drain from voids in specimens), designating this mass as B. Calculate the Gmb to three decimal places using the following formula:
GmbMeasured (at NDesign) = A
Example: Dry mass of specimen (A) = 4750.0 g SSD mass of specimen (B) = 4768.4 g Mass of specimen in water (C) = 2732.8 g
GmbMeasured (at NDesign) = 8.732,24.768,4
5.5.2 If the bulk specific gravity GmbMeasured of the two specimens deviates by more than 0.015, the results are considered suspect and a new set of specimens must be made from the remaining QA samples. 5.5.3 Average the GmbMeasured (at NDesign ) values for the two test specimens and use the results for the computation of air voids and VMA for the sample.
Rev. February 5, 2007 29
5.5.4 On the first day of production of a mix design, the Engineer may designate one of the retained samples for the Contractor to cool to ambient air temperature over night, heat in a 230F convection oven for two hours, and to quarter for testing. The Contractor shall then compact and test Gyratory specimens in accordance with Sections 5.4 and 5.5 of this manual, and develop a Bulk Specific Gravity Reheat Calibration Factor (BRCF). Determine the BRCF by the second day of production if the QA tests are being conducted on reheated samples to compare the average Gmb of an unreheated compacted sample to the average Gmb of a reheated compacted sample. The BRCF will be considered accurate for the entire production of a particular mix design, but may be repeated at the discretion of the Contractor or the Engineer. This factor is only used to correct reheated results to agree with the original results when tests are performed on reheated samples. Calculate the BRCF to four decimal places according to the following formula.
BRCF = )()(
If the comparison of the reheated Gmb to the original Gmb shows a difference of 0.005 or less, then a BRCF shall not be used. 5.5.5 Determine the corrected Gmb for reheated samples according to the following formula. Corrected Gmb = Gmb (Reheated) x BRCF
5.6 Maximum Specific Gravity, Gmm 5.6.1 Procedure. Determine two Gmm values for the sample according to the procedures of AASHTO T 209 as modified below. Average the two test values for calculations. If the values for the individual tests differ by more than 0.011, conduct additional tests to determine the correct value for Gmm. 22.214.171.124 Use the appropriate sample from Subsection 5.3.4 of this manual. The minimum specimen size shall be 2000 gm for 19 mm and 25 mm mixtures and 1500 gm for 9.5 mm and 12.5 mm mixtures. 126.96.36.199 Age the sample under the same conditions as the Gyratory specimens (Subsection 5.4.2).
Rev. February 5, 2007 30
188.8.131.52 Thoroughly break up the mixture and cool to ambient temperature, using care not to fracture the mineral particles, so that the particles of the fine-aggregate portion are not larger than 1/4-inch in diameter. The mixture is easiest to break apart after a brief cooling period while it is still warm. A portable electric fan may be used to speed the cooling process. 184.108.40.206 Calibrate metal bowls by weighing under water using the bowl option. The volume of the metal bowls may not be measured using the pycnometer method. 220.127.116.11 Place the entire amount of each sample in appropriate container and weigh to the nearest 0.1 gram. Add water at 772F to cover the sample by 1-1/4 to 2 inches. A few drops of a dilute (10%) liquid detergent (such as Joy or equivalent), to act as a wetting agent, may be added to the water to facilitate the release of entrapped air. 18.104.22.168 Remove entrapped air by subjecting the contents of the container to a partial vacuum which will result in 30 mm Hg or less absolute pressure for 152 minutes. Check the residual pressure in the container using a gage or closed end manometer with an accuracy of 3 mm, attached independently to the container. The container and contents shall be shaken vigorously at intervals of about two (2) minutes in order to assist the removal of air bubbles. A mechanical shaker may be used if test results are available from the Contractor that demonstrate that results approximately equal to hand shaking can be obtained (0.008). If the mixture is exposed to air after the vacuum is released, the test results are invalid and the vacuum procedure must be conducted again. 22.214.171.124 Volume Determination 126.96.36.199.1 Flask - Fill flask with water taking care to avoid adding air bubbles during this process (causes a low value of Gmm). Adjust the temperature of the added water such that the temperature of the water in the flask is 772F. Check the temperature of the water in the flask and weigh 101 minutes after the completion of the vacuum. Calculate the Gmm to three decimal places as follows: Without Dry Back Correction:
Gmm = EDA
With Dry Back Correction:
Gmm = EDA
Rev. February 5, 2007 31
Where: A = Dry Mass of Test Specimen in Grams A1 = SSD Mass of Test Specimen (Dry Back Mass) in Grams D = Calibration Mass of Flask Filled With Water in Grams E = Final Mass of Flask, Test Specimen and Water in Grams Example: A = 2048.4 g A1 = 2050.4 g D = 1856.0 g E = 3051.5 g Without Dry Back Correction:
Gmm = 5.30510.18564.2048
With Dry Back Correction:
Gmm = 5.30510.18564.2050
188.8.131.52.2 Bowl - Suspend the bowl and contents in water at 772F taking care to avoid adding air bubbles (causes a low value of Gmm). Weigh 101 minutes after the completion of the vacuum. For calculations, use the equations in Subsection 184.108.40.206.1 except the D mass is the mass of the bowl under water and the E mass is the mass of the sample and bowl under water.
220.127.116.11 When the dryback is required, drain water from sample, taking care to prevent loss of any mix. Spread sample in a thin layer in a tared pan before an electric fan to speed evaporation and removal of surface moisture. After the bottom of the pan is visibly dry, weigh at 15 minute intervals, and when the loss in weight is less than 0.5 g for this interval, the sample may be considered to be surface dry. The procedure requires about 2 hours and shall be accompanied by intermittent stirring of the sample. Conglomerations of mixture shall be broken up by hand. Water contained in the voids of a conglomeration cause an error in the test results (Gmm low). Care must be taken to prevent loss of particles of mixture. The dry back correction is defined as the Gmm calculated without the dry back minus the Gmm calculated with the dry back. Average the dry back correction for the two tests for each sample. The dry back correction will always be zero or a positive number. The above dry back procedure shall be conducted on the first two sets of samples tested. After that, the dry back shall only be conducted on every eighth test. For the first two samples, the dry back for test 1 shall be used to calculate Gmm for test 1.
Rev. February 5, 2007 32
The calculations for test 2 shall be the average dry back correction from tests 1 and 2. After the first two tests, the dry back correction shall be the average of all previous dry back tests. For subsequent days of production, use the dry back correction available at the start of the day for all tests conducted that day even if a new dryback correction is determined during the day. An example of the dry back correction calculations for a project is given on the attached dry back summary sheet (Figure 1). The correction shall be used as given in the following schedule: Day 1 Test 1 - Use dry back from test 1. Test 2 - Use average dry back from tests 1 and 2. Test 3 - Use average dry back from tests 1 and 2. Test 4 - Use average dry back from tests 1 and 2. Day 2 Test 5 - Use average dry back from tests 1 and 2. Test 6 - Use average dry back from tests 1 and 2. Test 7 - Use average dry back from tests 1 and 2. Day 3 Test 8 - Use average dry back from tests 1 and 2. Test 9 - Use average dry back from tests 1 and 2. Test 10 - Use average dry back from tests 1 and 2.* Test 11 - Use average dry back from tests 1 and 2.* Day 4 Test 12 - Use average dry back from tests 1, 2, and 10. Test 13 - Use average dry back from tests 1, 2, and 10.
(Example Maximum Specific Gravity Dry Back Correction Calculations)
Maximum Specific Gravity Dry Back Correction Summary Sheet
Day 1 1 2.508 2.505 0.003 0.003 1 0.003 2.505 2 2.508 2.503 0.005 0.008 2 0.004 2.504 3 2.518 - - - - 0.004 2.514 4 2.514 - - - - 0.004 2.510 Day 2 5 2.509 - - - - 0.004 2.505 6 2.503 - - - - 0.004 2.499 7 2.502 - - - - 0.004 2.498 Day 3 8 2.515 - - - - 0.004 2.511 9 2.505 - - - - 0.004 2.501 10 2.507 2.500 0.007 - 2* 0.004 2.503 11 2.504 - - - - 0.004 2.500 Day 4 12 2.501 - - 0.015 3 0.005 2.496 13 2.498 - - - - 0.005 2.493
Rev. February 5, 2007 33
18.104.22.168 On the first day of production of a mix design, the Engineer may designate one of the retained samples for the Contractor to cool to ambient air temperature overnight, heat in a 230F convection oven for two hours, and quarter for testing. The Contractor shall then determine the maximum specific gravity in accordance with Section 5.6 of this Manual and develop a reheat calibration factor. Determine the maximum specific gravity Reheat Correction Factor (MRCF) by the second day of production if the QA tests are being conducted on reheated samples to compare the average Gmm of an unreheated sample to the average Gmm of a reheated sample. The MRCF will be considered accurate for the entire production of a particular mix design, but may be repeated at the discretion of the Contractor or the Engineer in the field QC laboratory. This factor is only used to correct reheated results to agree with the original results when the tests are performed on reheated samples. If the comparison of the reheated Gmm to the original Gmm shows a difference of 0.005 or less, then a MRCF shall not be used. It is expected that the MRCF value will be less than 1.000. If the MRCF value is between 1.000 and 1.015, use 1.000. If above 1.015, retest. Calculate the MRCF to three decimal places using the following formula.
MRCF = )()(
22.214.171.124 Determine the corrected Gmm for reheated samples using the following formula: Corrected Gmm = Gmm (Reheated) x MRCF
5.7. Moisture Damage Testing
5.7.1 Tensile Strength Ratio, TSR. Conduct the TSR tests according to MT-63 on samples of HMA mixture from the plant. Test a minimum of four specimens (2 wet / 2 dry). The TSR specimens shall have a 150 mm diameter and should be approximately 95 mm in height. Divide the specimens into two groups of approximately equal voids in the required void range. The saturation procedure, soaking and strength tests may be conducted in an off site laboratory. The gyratory machine should be set to provide samples that are 95 mm in height. Use the following procedures to determine the approximate sample weight to provide the desired height. If the Gyratory Correction Factor for Mixture Sample is not determined for the sample obtained for TSR testing, use an approximate value based on recent Gyratory testing. It is recommended that a trial batch be produced to verify the estimated sample weight.
Rev. February 5, 2007 34
Mixture Data: Maximum Specific Gravity (Gmm) = 2.396 Calculate GmbEstimated required to produce sample with 7% air voids. GmbEstimated (at 7% air voids) = (93 x 2.396) / 100 = 2.228
Calculate the sample mass necessary to produce the 95 mm height for specimens with a diameter of 150 mm.
Sample Mass = 2.228 x 95 x 17.6715 = 3,740 g of mix. NOTE: 17.6715 is a constant for 150 mm specimens. 5.7.2 Boiling Water Test. Conduct boiling water tests according to MT-59 at least once per day of production. The extent of stripping (coating loss) is determined by visual examination of the sample and estimating the proportion of stripped particles. If the amount of stripped particles exceeds 5 percent, some modification of the mixture is required to reduce the potential for moisture damage (see Subsection 401.02.5.3 of the specifications).
5.8 Calculating Air Voids , Pa 5.8.1 The air void determination is a relationship between maximum specific gravity (Gmm) and the mixture bulk specific gravity [GmbMeasured (at NDesign)]. Air voids can be calculated for laboratory compacted specimens and sawed (or cored) specimens from compacted pavements. 5.8.2 Mixture air voids for each sample shall be calculated using the average of the two maximum specific gravity (Gmm) tests and the average of the two bulk specific gravity [GmbMeasured (at NDesign)] tests, according to the following formula (calculate to one decimal place):
Air Voids (Pa), % =
GGG )( x 100
Example: Gmm = 2.396 GmbMeasured (at NDesign) = 2.299
Air Voids (Pa), % = 396.2
100)299.2396.2( x = 4.0 %
Rev. February 5, 2007 35
5.9 Calculating Voids In Mineral Aggregate, VMA
5.9.1 The VMA measures the void spaces between the aggregate particles in a compacted paving mixture. The VMA includes the air voids and the effective asphalt content. It is expressed as a percent of the total volume of the mixture. 5.9.2 VMA is calculated using the combined aggregate bulk specific gravity (Gsb) for the aggregate blend from the mix design, the asphalt content determined on the sample (Pb), and the average compacted specimen bulk specific gravity of the two specimens at NDesign (GmbMeasured) according to the following formula (calculate to one decimal point):
VMA, % = 100 -
Example: Pb = 5.4 % GmbMeasured (at NDesign) = 2.299 Gsb = 2.574
VMA, % = 100 -
574.2)4.5100(299.2 x = 15.5
5.9.3 When any HMA plant aggregate cold feed bin percentage is changed by five percent or more from the job mix formula, calculate a new combined aggregate bulk specific gravity (Gsb) using the following formula:
Gsb = etc
Example: Aggregate #1 Gsb = 2.692 Percent = 30 Aggregate #2 Gsb = 2.524 Percent = 70
100 = 2.572
Rev. February 5, 2007 36
5.10 Gradation Of Extracted Aggregate From Mixture
5.10.1 Use appropriate sample from Subsection 5.3.4. 5.10.2 Perform the test in accordance with Mississippi Test Method MT-31.
5.11 Field Adjustment of Job-Mix Formula, JMF. The JMF may be adjusted in the field based on production test results according to the procedures in Subsection 4.2.3.
5.12 Documentation. Document all observations, records of inspections, adjustments to the mixture, and test results on a daily basis. Maintain a running average calculation for all tests listed in Subsection 126.96.36.199.7. If single tests are performed as a check on individual mixture properties, between regular samples, without performing all tests listed in Subsection 188.8.131.52.7, the results of those individual tests must not be included in the running average calculations for that particular property. Record the results of observations and records of inspection as they occur in a permanent field record. Record all process adjustments and job mix formula changes on the air void charts. Provide copies of all test data sheets and the QC test results on a form similar to MDOT Form TMD-005 to the Engineer on a daily basis (before 9:00 AM the day after production). Fourteen days after the completion of the project, provide the Engineer with the original testing records and control charts in a neat and orderly manner.
5.13 JMF Limits, Warning Limits and Warning Bands. JMF limits are the specified tolerances to the job mix formula beyond which the mixture is unacceptable and subject to removal. Warning limits are the specified tolerances to the job mix formula beyond which the mixture is unsatisfactory and subject to a price reduction. These limits serve as a warning to make adjustments before unacceptable mixture is produced. Warning bands are defined as the area between the warning limits and the JMF limits. The JMF limits and warning limits for the job mix formula are based on a running average of the last four test data points.
Rev. February 5, 2007 37
The specified JMF limits and warning limits are as given in Subsection 401.02.5.5 of the contract specifications.
5.14 Corrective Action. Document all corrective action and include all test values in the project records, in the running average calculations and on the control charts. Take corrective action according to the procedures required in Subsection 401.02.5.8 of the contract specifications. 5.14.1 Examples of Corrective Action. These examples are based on the following data: ABC Asphalt from Jackson, Mississippi was the successful bidder on a project that required approximately 10,000 tons of a ST 12.5 mm mixture. Assume that all density and aggregate testing met the project requirements. Copies of the Summary Report of QC Mixture Properties (Form TMD-006) and the appropriate QC Charts for each example are provided in Appendix 3. The mixture production records for the project were as follows:
Date Tons Produced 2/23 1,800 2/24 1,460 2/25 2,000 2/26 1,440 2/27 1,950 2/28 1,450 Total 10,100
184.108.40.206 Example 1. The Contractors production started out with the air voids slightly low and the asphalt binder content slightly high. The field density results were okay but just meeting the minimum specification. The Contractor was reluctant to change the mixture because of concern for possible field density problems. On 2/25 after test 7, the Contractor notified the MDOT QA person that the air voids were trending towards the warning limit. On 2/26 after test 9, the Contractor notified MDOT that the second running average for air voids exceeded the warning limits and that they planned to reduce the asphalt binder content by 0.2 percent to bring it in line with the design value and as a result, increase air voids. The reduction in asphalt binder content was dialed into the plant and production continued. The Contractor closely monitored the field density with a nuclear gauge and modified the number of roller passes to compensate for the mixture change. The running average for air voids at test 13 (four tests after the change was made) was back inside the warning limits. Based on the specification, the Contractor is paid at a pay factor of 1.0 for all the mix produced to that point. 220.127.116.11 Example 2. The Contractors production starts out with the air voids slightly low and the asphalt binder content slightly high. The field density results
Rev. February 5, 2007 38
were okay but just meeting the minimum specification. The Contractor was reluctant to change the mixture because of concern for possible field density problems. On 2/25 after test 6, the Contractor notified the MDOT QA person that the air voids were trending towards the warning limit. On 2/25 after test 8, the contractor notified MDOT that the second running average for air voids exceeded the warning limits. Production had already shut down for the day. The next morning prior to production, the Contractor notified MDOT that they planned to make a minor gradation change in an attempt to increase the VMA, which should also increase the air voids. The running average for air voids at test 12 (four tests after the change was made) was still in the warning bands. Production continued this way until 2/28 when the Contractor finally adjusted the asphalt binder content. Based on the specifications, the Contractor will receive reduced pay for unsatisfactory mixture from the plant tonnage at the stop point (second running average of four exceeds the warning limits) to the tonnage when the running average is back within the warning limits. For this project, the mixture subject to reduced payment includes 410 tons produced on 2/25 (stop point - 1,590 tons until the end of the day - 2,000 tons) all the tons produced on 2/26 and 2/27 and 349 tons produced on 2/28. The total quantity of mixture subject to reduced payment is 4,149 tons. The payment factor of 0.70 is determined according to the table in Subsection 401.02.6.3 of the contract specifications. 18.104.22.168 Example 3. The Contractors production starts out with the air voids slightly low and the asphalt binder content slightly high. The field density results were okay but just meeting the minimum specification. The Contractor was reluctant to change the mixture because of concern for possible field density problems. On 2/25 after test 6, the Contractor failed to notify the MDOT QA person that the air voids were trending towards the warning limit. On 2/25 after test 8, the Contractor ignored the fact that the second running average for air voids exceeded the warning limits and continued production. According to the specifications, failure to stop production and make the necessary adjustments when required shall subject all mixture produced from the stop point tonnage to the tonnage point when the running average is back within the warning limits to be considered unsatisfactory. For this example, the stop point is test 8 and the tonnage when the running average is back within the warning limits is test 14. As in the case of the previous example, this represents 4,149 tons of mixture. The payment factor of 0.70 is determined according to the table in Section 401.02.6.3 of the contract specifications. 22.214.171.124 Example 4. The Contractors production starts out with the air voids slightly low and the asphalt binder content slightly high. The field density results were okay but just meeting the minimum specification. On 2/26 at test 10, the individual test results for asphalt binder content and air voids exceeded 1.7 times the JMF limits. MDOT tested the retained sample for test 10 and confirmed the results within the allowable differences in Subsection 907-401.02.6.2 of the contract specifications. The Engineer investigated the problem and found that fat spots were apparent on the pavement and that roadway density was above 96 percent, both confirming high asphalt and low air voids. A review of plant operations indicated
Rev. February 5, 2007 39
that the asphalt pump malfunctioned approximate two truck loads prior to test 10 and continued for the rest of the day. This represented 30 tons for the two trucks plus the 206 tons to complete the day (test point - 1,234 tons until end of day - 1440 tons). Because this mixture was placed in a busy intersection, the Engineer required the 236 tons of mixture to be removed and replaced at no additional cost to the state.
5.15 Trouble Shooting 5.15.1 Effective Specific Gravity (Gse). The calculation of the effective specific gravity will provide a useful tool to the Quality Control Technician. The effective specific gravity is calculated primarily from the maximum specific gravity (Gmm) of a sample and the asphalt content (Pb). It defines the relationship between the weight of the aggregate and the bulk volume of the aggregate minus the volume of absorbed asphalt. The effective specific gravity should be a constant for most Mississippi mixtures. It will change however, if the specific gravity of one of the major aggregate components change or if the proportion of aggregates with different specific gravities in the blend change. For most QMP projects, changes in the effective specific gravity will result from errors in testing or sampling for Gmm or Pb determinations. When deviations exceeding 0.012 occur in the effective specific gravity, check test results against previous data and verify that testing is correct. The Gse value is calculated using the following equation:
Where: Pb = Percent of Asphalt Binder in Sample Gmm = Maximum Specific Gravity of Sample Gb = Specific Gravity of Asphalt Binder at 77F / 77F (typical value approximately 1.030) Example: Pb = 5.4 Gmm = 2.396 Gb = 1.034
Rev. February 5, 2007 40
5.15.2 Changes in Mixture Volumetrics. The volumetric properties of a mixture are normally defined as the air voids (Pa) and the voids in the mineral aggregate (VMA). The air voids for a given compaction level are controlled by the asphalt binder content and the VMA of the mixture. If the asphalt binder content remains constant, changes in the mixture VMA will cause a corresponding change in the mixture air voids. An increase in the asphalt binder content of 0.1 percent can be expected to lower the air voids by approximately 0.25 percent if everything else remains approximately the same. The VMA of a mixture for a given compaction level is controlled by the gradation and shape of the aggregate. For most mixtures, we can assume that the shape of the component aggregate will remain constant. The dust proportion of the gradation [material passing the No. 200 sieve] has by far the greatest influence on the VMA. A one percent increase in dust in the mixture will lower the VMA by approximately 0.9 percent. Control of the dust at a HMA plant is of primary importance during a QMP project. Studies have found that a number of HMA plants equipped with baghouses generate more dust than what is contained in the cold feed aggregates. A number of Contractors are adding extra dust to the mixture design to compensate for this.
Rev. February 5, 2007 41
CHAPTER 6 MDOT QUALITY ASSURANCE PROGRAM
6.1 Materials Samples
6.1.1 Asphalt Binder Material. Procedures for acceptance of asphalt binder are set out in Section 2.1.2 of the Materials Division Inspection, Testing and Certification Manual. Obtain random samples of asphalt binder from the Contractor at the minimum frequency of one per 100,000 gallons. Samples are to be obtained from the Contractors working tank in accordance with AASHTO T 40 and ASTM D 3665. Submit samples to the District Laboratory in sealed one quart metal containers for testing under AASHTO T 316. Obtain a random sample of asphalt binder at the minimum frequency of one per 200,000 gallons, and submit to the Materials Division for testing under AASHTO T 315. Immediately upon determining that a sample of asphalt binder fails to conform to specification requirements, notify the Contractor and asphalt supplier. The Contractor is to suspend operations immediately. The Contractor along with the asphalt supplier must determine the cause and take appropriate action to correct the problem. The Contractor may resume operations after the problem has been corrected. Determine the acceptability of any mixture placed with the non-complying asphalt binder in accordance with Subsection 105.03 of the Mississippi Standard Specifications for Roads and Bridge Construction. 6.1.2 Hydrated Lime. As a minimum, obtain one sample (one quart in size) of hydrated lime per project. If the source changes or there is a suspected problem, resample. Sample hydrated lime from the Contractors storage tank in accordance with AASHTO T 218. Place sample in a sealed one quart metal container, and submit to the Materials Division for testing.
6.2 HMA Quality Assurance Requirements. 6.2.1 General. Acceptance for mixture quality (VMA and air voids @ NDesign, gradation, and asphalt content) is based on the Contractors QC test results performed as set out in Chapter 5 of this manual, and verified by MDOTs QA program as set out below. 6.2.2 Samples. As a part of the QA program, verification tests will be performed on samples taken by the Contractor under the direct supervision of the Engineer at a time specified by the Engineer. The Contractors split portion of the QA verification sample will not be included in the QC running average. However, the test results should be retained for the dispute resolution process (See MDOT HMA QC/QA Dispute Resolution Flow Chart).
Rev. February 5, 2007 42
6.2.3 Testing Frequency. QA verification testing frequency must be equal to or greater than 10 percent of the tests required for Contractor QC. At least one sample must be tested from the first two days of production. When a problem develops on the project such that an investigation is conducted to resolve testing differences, the District will increase sampling frequency to the same frequency required for Contractor testing until the problem is resolved. Any or all of the Contractor retained samples may be tested as necessary for validation of Contractor QC test results and mixture quality. The Contractor is required to keep the retained QA split samples (A+D) for 14 calendar days from the date of sampling (401.02.5.3(j)). 6.2.4 Quality Assurance Verification Testing. Perform the tests in accordance with procedures contained in Chapter 5 of this manual. Round all test results in accordance with Subsection 700.04 of the Mississippi Standard Specifications for Road and Bridge Construction. All testing and data analysis for QA must be performed by a CAT-I Technician or by an assistant under the direct supervision of the CAT-I Technician. For maximum specific gravity testing, verify the Contractors dryback procedure on the first sample tested by MDOT. If the MDOT dryback correction is within 25 % of the Contractors value, future MDOT testing may use the Contractors value. If the dryback values are not within the above tolerance, find out why the problem exists and continue MDOT dryback testing until the results agree. Provide the test results to the Contractor within two asphalt production days after the sample has been obtained. 6.2.5 Validation of Quality Control Test Results. For the Contractors QC test results to be used in making the acceptance decision, the average of the previous four (4) QC tests must compare to the QA verification test result and the QA verification test results must meet mixture JMF production requirements. If four QC tests have not been tested at the time of the first verification test, the verification test results will be compared to the average of the preceding QC tests (one, two or three tests). If the verification test is the first material tested on the project or if a significant process adjustment (one that is expected to change the test results) was made just prior to the verification test, the verification test results will be compared to the average of four subsequent QC test results. For all other cases after a significant process adjustment, the verification test results will be compared to the average of the preceding QC tests (taken after the adjustment) as in the case of a new project start-up when four QC tests are not available. In the event that the above comparison of test results is outside the allowable differences (Subsection 907-401.02.6.2 of the contract specifications), or the QA
Rev. February 5, 2007 43
verification test results fail to meet the JMF specification requirements for asphalt content, air voids or VMA, investigate the reason immediately. The investigation may include testing of the retained QA split samples (A+D), review and observation of the Contractor's testing procedures and equipment, and a comparison of split sample test results by the Contractors QC laboratory, the Districts QA laboratory, and the Materials Division. See Section 6.6 of this manual for a guideline on conducting the investigation. If reasons for the differences cannot be determined or if the Contractors tests are proven incorrect, the QA verification test results will be used in place of the QC data and the appropriate payment for the HMA will be based on the Specifications (401.02.6.3). Periodically witness the sampling and testing being performed by the Contractor. Promptly notify the Contractor both verbally and in writing of any observed deficiencies (evaluation forms contained in the appendix may be used for this purpose). When differences in procedures exist between the Contractor and the Engineer which cannot be resolved, a decision on which procedure is correct will be made by the State Materials Engineer, acting as the referee. The Contractor will be promptly notified in writing of the decision. If the deficiencies are not corrected, the Engineer will stop production until corrective action is taken.
6.3 HMA Plant Production Review Guidelines. The District QA program shall follow the following guidelines: 6.3.1 Prestart-up. The District Materials Section should supply the QA team with:
The lab number of the aggregate quality test reports for the aggregate sources being used.
A copy of the Contractor's mix design and the Tentatively Approved (TMD-042) mix design report from the Materials Division.
The contract special provisions. The quality assurance team should:
Verify that the QC team personnel have the proper certifications. Verify that the HMA mixing plant inspection has been accomplished as per
Section 1.1.2 of the Materials Division Inspection, Testing and Certification Manual and that the automatic plant control systems are functioning.
Review QC and QA equipment calibration data as required in Section 3.2 of this manual to determine that calibrations are up to date (according to AASHTO R 18) and determine if the following equipment complies with the appropriate specifications:
Rev. February 5, 2007 44
Balances (QA team check with known weight) Gyratory compactor-Ensure inside diameter of gyratory molds meets tolerances specified in Section 4.2 of AASHTO T 312. Molds found to be outside the tolerance should be discarded. Vacuum pumps, hoses, bowl or flask, manometer gauge and hookup, etc. Water baths, thermometers, ovens Fax and copy machine
Review with the QC teams proposed sampling locations and splitting procedures.
Review procedure for determining the reheat correction factors for Gmb and Gmm and the dryback correction procedure.
Verify that the Hydrated Lime feed system meets the requirements of 401.03.2.1.1 and 401.03.2.1.2 and that the Contractor has the required hydrated lime inventory (401.02.3.1).
6.3.2 Start-up Day. A member of the District QA team should be at the QC laboratory on start-up day. This person should:
Verify that the Contractor is producing the Tentatively Approved mixture design.
Verify the source of supply of the asphalt binder. Materials from different sources should not be mixed without prior written approval of the Engineer (401.03.2.1.5).
Verify that the maximum amount of material being fed through a single cold feed is 45 percent (401.03.2.1.2).
Verify that the RAP scalping screen is in place and functioning (401.02.3.1). Observe sampling and splitting procedures. Observe testing procedures including reducing the field sample to testing size. Check nuclear asphalt content gauge calibration using standard pan or verify
that the incinerator oven has been properly calibrated. Verify that the mixture moisture content determined for correcting the asphalt
content meets the requirements of 401.03.2.1.3. Review data calculations to include:
Asphalt content (Pb). Mix air voids (Pa). Voids in the Mineral Aggregate (VMA). Running average (if applicable).
Compare Contractor process control data with the Job Mix Formula (JMF) data as soon as possible (voids, VMA, Gmm, Gmb, asphalt content and gradation).
Rev. February 5, 2007 45
Arrange to have a verification sample tested by the QA team and compare results with the QC data as soon as possible. These sample test results may be used as one of the required 10% QA verification tests. Designate one of the retained samples for the Contractor to use for determining reheat correction factors if appropriate. 6.3.3 During Production. Periodically witness the sampling and testing being performed by the Contractor. Promptly notify the Contractor both verbally and in writing of any observed deficiencies. Use the evaluation forms (QMP Inspectors Checklist) in the Appendix to document any observed testing deficiencies. Have the Contractors technician sign a copy of the evaluation form. Review the plant production requirements.
Verify that the Contractor is producing the Tentatively Approved mixtur